In this paper, we focus on current–voltage (I–V) characteristics in several kinds of quasi-one-dimensional (quasi-1D) nanofibers to investigate their electronic transport properties covering a wide temperature range from 300 down to 2 K. Since the complex structures composed of ordered conductive regions in series with disordered barriers in conducting polymer nanotubes/wires and CdS nanowires, all measured nonlinearI–Vcharacteristics show temperature and field-dependent features and are well fitted to the extended fluctuation-induced tunneling and thermal excitation model (Kaiser expression). However, we find that there are surprisingly similar deviations emerged between theI–Vdata and fitting curves at the low bias voltages and low temperatures, which can be possibly ascribed to the electron–electron interaction in such quasi-1D systems with inhomogeneous nanostructures.
Keywords:Conducting polymers; I–Vcharacteristics; FIT model; Nanowires/tubes
Recently, low-dimensional materials especially nanowires and nanotubes have attracted considerable attention in view of their novel features and electronic device applications in future [1-3]. The unusual electronic transport properties in conducting chemically doped polymers have been widely investigated and reported owing to their unique structural features, which are known to be very inhomogeneous; namely, in some regions, the polymer chains are ordered, and in other regions, the chains are disordered [4-6]. This complex structure in disordered materials including doped polymer and inorganic nanofibers is generally considered as conduction regions or long conducting pathways separated by small insulating barriers. Especially, as a key indicator to electrical behavior, novel nonlinear current–voltage (I–V) characteristics with temperature and field-dependent features are observed in such quasi-one-dimensional (quasi-1D) inhomogeneous structures [7-13]. In particular, Kaiser et al. [11,12] recently proposed a generic expression (extended fluctuation-induced tunneling (FIT)  and thermal excitation model) for the nonlinear I–V characteristics based on numerical calculations for metallic conduction interrupted by small barriers and showed that the expression can give a very good description to the temperature and field-dependent nonlinearities of I–V curves in polyacetylene nanofibers, vanadium pentoxide nanofibers, etc.
The electronic density of states (DOS) near the Fermi energy EF is known as an important physical quantity for understanding the electronic transport mechanism in strongly localized systems  where the electron–electron interaction (EEI) is first showed with created depletion in DOS near EF by Pollak  and Srinivasan . Efros and Schklovskii [17,18] called this depletion “Coulomb gap,” which can strongly affect the transport properties. Furthermore, it is reported that the electron states in doped nanofibers are more localized by disorder at low temperature . However, most of conduction electrons are considered as delocalized and free to move over a very large distance compared to atomic dimension in FIT regime , the EEI is not considered. Thus, if taking the EEI into account, is Kaiser expression still generic for nonlinear I–V characteristics of quasi-1D material? In this paper, the I–V characteristics of a series of doped polymer nanofibers and helically twisted CdS nanowire ropes are measured by a standard two-probe method covering a wide temperature range to investigate the transport behavior and figure out this open question. We find all these I–V characteristics show similar nonlinear features and are well fitted to Kaiser expression. However, the surprisingly similar deviations between the I–V data and fitting curves emerge in low-field region at low temperatures, which have not been reported and discussed before.
8-Hydroxyquinoline-5-sulfonic acid doped polypyrrole (PPY-HQSA) nanotubes and camphor-sulfonic acid doped polyaniline (PANI-CSA) nanotubes were prepared by a template-free self-assembly method . The tubular morphology of polypyrrole and polyaniline nanotubes was confirmed by a transmission electron microscopic (TEM) with outer diameters about 100–120 nm as shown in Figs. 1a and 4a, separately. Conducting poly(3, 4-ethylenedioxythiophene) (PEDOT) nanowires with diameters about 95 nm (as shown in Fig. 3a) were prepared by a hard template method described in Refs. [19-21]. As shown in Fig. 2a, helically twisted CdS nanowire ropes composed of nanowires with diameters about 6–10 nm were synthesized by aqueous chemical growth method [22,23].
Figure 1. aTypical TEM image of polypyrrole nanotubes andbthe correspondingI–Vcharacteristics with fitting curves to Eq. 3measured from 300 down to 15 K
Figure 2. aTypical TEM image of CdS nanowire ropes andbthe correspondingI–Vcharacteristics with fitting curves to Eq. 3from 200 down to 60 K
The Pt microleads attached on isolated nanofibers were fabricated by focused-ion beam deposition. The detailed procedure can be found in previous publications [6,21-24]. The I–V characteristics of individual polypyrrole nanotube, helically twisted CdS nanowire rope, PEDOT nanowire and polyaniline nanotube were measured by scanning the voltage from −6 to 6 V with a step of 0.03 V using a Physical Property Measurement System from Quantum Design and a Keithley 6487 picoammeter/voltage source over a wide temperature range from 300 to 2 K. Here, it is noted that since the low-temperature resistance of the measured polypyrrole tube and CdS nanorope is very large, and thus, the corresponding current is very small (~ pA), their I–V curves are only measured above 15 and 60 K, separately.
Since the complex structure of disordered materials generally considered as conduction regions or long conducting pathways separated by small insulating barriers, the FIT conduction mechanism, proposed by Sheng , characterizes electrons transfer across the insulating barriers, which can be directly influenced by the voltage fluctuations in the conducting pathways. The mean current density through a barrier when a field Ea is applied across it is evaluated as
where P(ET) is the probability that the fluctuation field across the junction has the value ET (which may be in either direction). The tunnelling current j(E) for a total field Eb = (Ea + ET) in the barrier is denoted as
where m and ε are the carrier mass and energy, respectively. In terms of the structure features of quasi-1D disordered materials and the FIT model , Kaiser et al. [11,12] proposed a generic expression, which can give a good description to the changing shape of nonlinear I–V characteristics in quasi-1D systems by performing numerical calculations of the current fluctuation-assisted tunnelling through conduction barriers and thermal activation over the barriers:
where G0h, and V0 are parameters. G0 is the temperature-dependent low-field (V → 0) conductance. The parameter h = G0/Gh (h < 1) yields a decrease of G below the exponential increase at higher voltages V (Gh is the saturated conductance at a high-field value). V0 is a voltage scale factor, which gives an exponential increase in conductance as V increases depending strongly on the barrier energy. More details can be found in Refs. [11,12].
Comparison with Experiment
Kaiser et al. [11,12] has shown that the above expression can give a very good description to the observed nonlinearities in polyacetylene nanofibres, carbon nanotube networks, vanadium pentoxide nanofibres, and granular Sr2FeMoO6. In the present case, a series of I–V characteristics at different temperatures with fitting curves to Kaiser generic expression Eq. 3 are shown in Figs. 1(b), 2(b), 3(b), and 4(b). We note that all these I–V characteristics are essentially symmetric upon reversal of the voltage direction, so only positive voltages are used to show the fits more clearly.
Figure 3. aTypical TEM image of single PEDOT nanowire andbthe correspondingI–Vcharacteristics with fitting curves to Eq. 3from 80 down to 2 K
Figure 4. aTypical TEM image of polyaniline nanotubes andbthe correspondingI–Vcharacteristics with fitting curves to Eq. 3from 250 down to 3 K
Figure 1b shows the typical nonlinearI–Vcharacteristics of single polypyrrole nanotube with diameter about 100 nm. With increasing temperature and voltage, the nonlinearity decreases and the ohmic component become dominant. The nonlinearI–Vcharacteristics can be well fitted to Eq. 3and the fitting parameters at some selected temperatures are shown in Table 1In this case, the low-field conductanceG0increases substantially from 0.0071 to 52.932 nS as temperature increases from 15 to 250 K. The parameterhincreases from 0.0065 to 0.6805 with increasing temperature corresponding to a decrease ofGbelow the exponential increase at higher voltages as shown in Fig. 1b. The voltage scale factorV0also increase from 1.0685 V atT = 15 K to 6.9725 V atT = 250 K, indicating a lessening of nonlinearity in theI–Vcharacteristics as temperature increases. It is about 160 K where linear component becomes dominant in this case.
Table 1. Fitting parameters to Eq. 3for polypyrrole nanotube at different temperatures
The similar highly nonlinearI–Vcharacteristics of CdS nanorope are shown in Fig. 2b. Although the nonlinearity decreases with increasing temperature, the plot is still highly nonlinear even atT = 200 K. In this case, the nonlinearities at higher temperatures indicate larger barrier energies than that for the polypyrrole nanotube. It can be seen from the fits in Fig. 2b that Kaiser expression can give a good account to the temperature and field-dependent nonlinearities. The fitting parameters are shown in Table 2The low-field conductanceG0shows weaker increase with temperature than that for the polypyrrole case.hhas smaller values indicating a higher exponential increase inGwith increasing temperature (h = 0.1052 at T = 200 K). The voltage scale parameterV0also varies in a small range from 1.838 V atT = 60 K to 1.8558 atT = 200 K than that for the polypyrrole tube, reflecting the smaller change in nonlinearities ofI–Vcharacteristics.
Table 2. Fitting parameters to Eq. 3for CdS nanorope from 200 down to 60 K
As shown in Fig. 3b, the measuredI–Vcharacteristics of single PEDOT nanowire from 80 down to 2 K show a much more linearity compared with that of polypyrrole nanotube in Fig. 1b and CdS nanorope in Fig. 2b. All these data for PEDOT nanowire can be well fitted to Eq. 3(as shown in Fig. 3b) with fitting parameters given in Table 3The low-field conductanceG0shows higher values and increases substantially as temperatureTincreases. Linearity becomes dominant inI–Vcharacteristics at a lower temperature about 50–80 K reflecting smaller barrier energy in the PEDOT nanowire. The more linearI–Vcharacteristics than the foregoing two cases yield larger values in the fitting parametershand smaller values in the voltage scale parameterV0as shown in Table 3. In addition, as shown in Fig. 4b, the similarI–Vcharacteristics are also observed in single polyaniline nanotube with diameter about 120 nm with fitting parameters given in Table 4.
Table 3. Fitting parameters to Eq. 3for PEDOT nanowire from 80 down to 2 K
Table 4. Fitting parameters to Eq. 3for polyaniline nanotube from 250 down to 3 K
Thus, based on our experimental results as shown from Figs. 123, and 4, we conclude that the FIT model and Kaiser expression can give a very good explanation to the electronic transport properties and the nonlinear I–V characteristics in quasi-1D materials in accordance with previous reports [11,12]. In FIT regime, most of delocalized and free conduction electrons compared to atomic dimension in disordered materials transfer across the insulating gaps in the conducting pathways . In terms of Kaiser expression, considering the complex structures composed of ordered metallic regions in series with disordered conduction barriers in such quasi-1D systems, essentially, the nonlinear I–V behavior corresponds to tunneling through barriers with thermal fluctuations considerably smaller than the barrier height. As temperature increase, the thermal energy becomes comparable to the barrier height and linearity becomes dominant. Besides temperature, the nonlinearity also shows field-dependent feature. As the bias voltage increases, the difference in Fermi levels between two sides of barriers is comparable to the barrier energy, then the conductance will saturate at a value Gh and the I–V curves will become linear.
Here, we should note that the I–V characteristics, which are linear–linear plotted in Figs. 1(b), 2(b), 3(b), and 4(b), as well as in Refs. [11,12], cannot show the low-field region clearly, so log-linear plots are adopted instead of linear-linear plots, which are shown in Fig. 5(a)–(d), separately. The surprisingly similar deviations between the I–V data and fitting curves emerge in low-field region at low temperatures, which have not been reported and discussed. According to the theory developed by Pollak, Efros, and Schklovskii and coworkers [15-18], the strong EEI creates a Coulomb gap in DOS near Fermi level in localized systems. By now, there have been a lot of experimental evidences in which hopping is indeed influenced by the presence of Coulomb gap at sufficiently low temperatures [6,24-30]. For instance, the EEI can result in a smooth crossover from three-/two-dimensional Mott to Efros–Shklovskii variable-range hopping conduction [6,25-28] and Coulomb gap-like structure in dI/dV curves [26-30]. In addition, our previous studies on conducting polyaniline, polypyrrole, and PEDOT nanotubes/wires have indicated that the quasi-1D nanostructures are composed of crystalline regions and amorphous regions [6,31,32], and the EEI may be enhanced and dominate the low-temperature electronic transport behavior [6,24,29]. Therefore, we suggest that the observed small deviations in Fig. 5(a)–(d) could be possibly due to the EEI, which has not been included in Kaiser expression or FIT model and should be taken into account especially at low temperatures in quasi-1D systems where electron states are more localized due to confinement effect or disorder. However, further theoretical and experimental investigations are needed to clarify this point.
Figure 5. The corresponding log-linear plot of theI–Vcharacteristics forapolypyrrole nanotube,bCdS nanorope,cPEDOT nanowire, anddpolyaniline nanotube
In summary, the electronic transport properties in several kinds of individual polymer nanofibers and CdS nanoropes were measured and investigated covering a wide temperature range. All these quasi-1D materials show similar temperature and field-dependentI–Vcharacteristics, which are well fitted to the extended FIT and thermal activation conduction model (Kaiser expression) consistent with the complex structures composed of ordered metallic region in series with disordered conduction barriers in such quasi-1D systems. We conclude that Kaiser expression is a possible way to explain the electrical behavior at relatively high temperatures and propose that the deviations emerged in low-field region at low temperatures are possibly due to the enhanced EEI in quasi-1D nanofibers with nanoscale inhomogeneous structures.
This work was financially supported by the National Natural Science Foundation of China (Grant No 10604038) and the Program for New Century Excellent Talents in University of China (Grant No NCET-07-0472).
Rev. Mod. Phys.. 2001, 73:701.
COI number [1:CAS:528:DC%2BD3MXptVyhtL8%3D]; Bibcode number [2001RvMP...73..701M]Publisher Full Text
Chem. Rev.. 2007, 107:2891.
COI number [1:CAS:528:DC%2BD2sXmslyrurc%3D]PubMed Abstract | Publisher Full Text
Phys. Rev. B. 1998, 57:9567.
COI number [1:CAS:528:DyaK1cXisVGhtrY%3D]Publisher Full Text
Phys. Rev. B. 2005, 72:024213.
Bibcode number [2005PhRvB..72b4213Z]Publisher Full Text
Phys. Rev. B. 2005, 71:165412.
Bibcode number [2005PhRvB..71p5412L]Publisher Full Text
Phys. Rev. B. 2005, 72:153202.
Bibcode number [2005PhRvB..72o3202A]Publisher Full Text
Synth. Met.. 2005, 152:497.
COI number [1:CAS:528:DC%2BD2MXpvVGksL0%3D]Publisher Full Text
Phys. Rev. B. 2007, 76:115415.
Bibcode number [2007PhRvB..76k5415G]Publisher Full Text
Phys. Rev. B. 2007, 76:045110.
Bibcode number [2007PhRvB..76d5110R]Publisher Full Text
Mol. Cryst. Liq. Cryst.. 2004, 415:115.
COI number [1:CAS:528:DC%2BD2cXotlehtLY%3D]Publisher Full Text
Synth. Met.. 2005, 152:181.
COI number [1:CAS:528:DC%2BD2MXpvVGlsbg%3D]Publisher Full Text
Phys. Rev. B. 1980, 21:2180.
COI number [1:CAS:528:DyaL3cXitVOmsrg%3D]; Bibcode number [1980PhRvB..21.2180S]Publisher Full Text
Phys. Rev. Lett.. 2001, 86:1845.
COI number [1:CAS:528:DC%2BD3MXhsVWltbo%3D]; Bibcode number [2001PhRvL..86.1845S]PubMed Abstract | Publisher Full Text
Discuss. Faraday Soc.. 1970, 50:13. Publisher Full Text
Phys. Rev. B. 1971, 4:2581.
Bibcode number [1971PhRvB...4.2581S]Publisher Full Text
J. Phys. C. 1975, 8:L49.
COI number [1:CAS:528:DyaE2MXhs1ersL8%3D]Publisher Full Text
Appl. Phys. Lett. 2007, 90:102114.
Bibcode number [2007ApPhL..90j2114D]Publisher Full Text
Int. J. Nanotechnol.. 2008, 5:838.
COI number [1:CAS:528:DC%2BD1cXps1Sktb8%3D]Publisher Full Text
Nanotechnology. 2006, 17:5903.
COI number [1:CAS:528:DC%2BD2sXhsFajsbY%3D]; Bibcode number [2006Nanot..17.5903L]Publisher Full Text
Appl. Phys. Lett.. 2005, 87:193109.
Bibcode number [2005ApPhL..87s3109W]Publisher Full Text
Chin. Phys. B. 2008, 17:1389.
COI number [1:CAS:528:DC%2BD1cXht12htrjK]Publisher Full Text
Nanotechnology. 2008, 19:215708.
Bibcode number [2008Nanot..19u5708L]PubMed Abstract | Publisher Full Text
J. Appl. Phys.. 1998, 84:806.
COI number [1:CAS:528:DyaK1cXktlOgtr0%3D]; Bibcode number [1998JAP....84..806G]Publisher Full Text
Appl. Phys. Lett.. 2006, 89:153132.
Bibcode number [2006ApPhL..89o3132S]Publisher Full Text
Chin. Phys. Lett.. 2008, 25:3474.
COI number [1:CAS:528:DC%2BD1cXhtF2hsr7L]; Bibcode number [2008ChPhL..25.3474L]Publisher Full Text
Nanotechnology. 2005, 16:746.
COI number [1:CAS:528:DC%2BD2MXnsl2msLc%3D]; Bibcode number [2005Nanot..16..746M]Publisher Full Text
J. Phys. Condens. Matter. 2004, 16:1123.
COI number [1:CAS:528:DC%2BD2cXktlOrt7c%3D]; Bibcode number [2004JPCM...16.1123L]Publisher Full Text
J. Phys. Chem. B. 2006, 110:23228.
COI number [1:CAS:528:DC%2BD28XhtVyhtr3O]PubMed Abstract | Publisher Full Text